Fracture resistance of endodontically treated teeth restored with a bulkfill flowable material and a resin composite Almira Isufi, DDS, PhD1 Gianluca Plotino, DDS, PhD1 Nicola Maria Grande, DDS, PhD2 Pietro Ioppolo3 Luca Testarelli, DDS, PhD1 Rossella Bedini3 Dina Al-Sudani, DDS4 Gianluca Gambarini, MD, DDS1
Endodontics Unit, Department of Oral and MaxilloFacial Sciences, “Sapienza” University of Rome, Italy 2 Department of Endodontics, Catholic University of Sacred Heart, Rome, Italy 3 Istituto Superiore di Sanità, Technology and Health Department, Rome, Italy 4 Department of Restorative Dental Sciences, College of Dentistry, King Saud University, Riyadh, Saudi Arabia
Corresponding author: Almira Isufi Endodontics Unit, Department of Oral and MaxilloFacial Sciences, “Sapienza” University of Rome Via Caserta 6 00161 Rome, Italy E-mail: [email protected]
Summary Aim. To determine and compare the fracture resistance of endodontically treated teeth restored with a bulk fill flowable material (SDR) and a traditional resin composite. Methods. Thirty maxillary and 30 mandibular first molars were selected based on similar dimensions. After cleaning, shaping and filling of the root canals and adhesive procedures, specimens were assigned to 3 subgroups for each tooth type (n=10): Group A: control group, including intact teeth; Group B: access cavities were restored with a traditional resin composite (EsthetX; Dentsply-Italy, Rome, Italy); Group C: access cavities were restored with a bulk fill flowable composite (SDR; Dentsply-Italy), except 1.5 mm layer of the occlusal surface that was restored with the same resin composite as Group B. The specimens were subjected to compressive force in a material static-testing machine until fracture occurred, the maximum fracture load of the specimens was measured (N) and the type of fracture
was recorded as favorable or unfavorable. Data were statistically analyzed with one-way analysis of variance (ANOVA) and Bonferroni tests (P .05).
Annali di Stomatologia 2016;VII (1-2): 4-10
A. Isufi et al.
60.8% of the failures in total were unfavorable (Group B 70%; Group C, 75%; control group, 25%). No significant differences were found in the mode of failure of the differently restored teeth between Group B and Group C, while intact teeth presented significantly more favorable fractures compared to restored specimens (both Group B and Group C).
Discussion The null hypothesis investigated in the present study can be rejected, as the results obtained support that there is no difference in the fracture resistance and in the mode of failure between endodontically treated maxillary and mandibular molars restored with a bulk fill flowable resin composite (SDR) or a traditional resin composite. Fracture susceptibility of root-filled teeth is affected mostly by the amount of the remaining dentin (4, 37) and it is not related to its biomechanical properties after endodontic treatment, such as hardness and toughness (38). Some studies have shown that the reduction of tooth structure results in weaker teeth due to restorative procedures (6-8). However, according to Reeh et al. (4), endodontic procedures have only a small effect on the tooth, reducing the relative rigidity by 5%, which is contributed entirely by the access opening. Restorative procedures and, particularly, the loss of marginal ridge integrity, were the greatest contributors to loss of tooth resistance. The loss of 1 marginal ridge resulted in a 46% loss in tooth rigidity, and a MOD preparation resulted in an average loss of 63% in relative cuspal rigidity. Several studies were conducted to determine the ideal materials and techniques to restore endodontically treated teeth because their long-term prognosis depends on the quality of the final restoration (39-42). Usually, to restore endodontically treated teeth several resin increments are required to fill the cavity preparation because of the large volume of the restoration. Thus, the clinician must compensate the polymerization shrinkage of traditional resin-based composite, by filling the cavities in several increments (43). A new category of flowable resin-based composites has been introduced as bulk fill base material that can be applied in 4 mm thick bulks instead of using the incremental placement technique, without negatively affecting the polymerization shrinkage, cavity adaptation or the degree of conversion (30). The results of the present study show that there were no significant differences in the static fracture resistance of endodontically treated molars restored with bulk fill flowable resin composite (SDR) and a traditional resin composite. Moreover, the mean fracture load for teeth restored with SDR was higher compared with the mean fracture load of specimens restored with traditional resin composites, without any statistical significance. Furthermore, the results of this study showed that there was no significant difference between teeth restored with SDR and intact
teeth. These findings may be attributed to the elastic buffer effect of using low viscosity flowable composite and the characteristic low contraction stress and low modulus of elasticity of SDR flow (44, 45). High flexural modulus can inhibit the ability of a material to resist deformation due to loading and promote the accumulation of surface and bulk defects, which may lead to premature failure (46, 47). These findings are in agreement with those of Atiyah et al. (48), who reported increased fracture resistance of endodontically treated premolars restored with SDR. In the present study 75% of the samples in the intact control teeth presented favorable fracture type that was an important statistical difference with the restored groups. In fact, the majority of the teeth restored with SDR (75%) and with a traditional resin composite (70%) reported unfavorable type of fracture. However, no significant differences were found in the mode of failure between restored teeth. Furthermore, all failures of the restored teeth were cohesive fractures, regardless of the type of restoration. The low elastic modulus may explain the severity of fracture type presented in restored teeth groups and the occurrence of unfavorable fracture. These findings are in agreement with previous reports that found an increased frequency and severity of cuspal fracture due to removal of cervical dentin (49). The limitations of this study must be recognized. The experimental methods used for in vitro analyses do not accurately reflect intraoral conditions, in which failures occur primarily due to fatigue. Future research in this area should use cyclic loading and other fatiguing simulation to more accurately reproduce the clinical environment. Additional clinical studies are necessary to determine the long-term prognosis of endodontically treated maxillary and mandibular molars restored with bulk fill flowable resin composite. Within the limitations of this in vitro study, endodontically treated upper and lower molars restored with bulk fill flowable resin composite presented a resistance to fracture under simulated compressive force not significantly different than that of traditional resin composite restorations. Restored teeth showed no significant decrease in fracture resistance compared to intact specimens. Furthermore, no differences were found in the mode of failure of the differently restored teeth, while intact teeth presented statistically more favorable fractures. Bulk fill flowable composites can be used to restore endodontically treated posterior teeth using 4 mm maximum increments and 1.5 mm occlusal traditional layer because this does not reduce the mechanical resistance of the restored teeth, while making the procedure easier, less stressful and with a reduced chair side time.
Acknowledgements The Authors deny any conflicts of interest. The Authors affirm that we have no financial affiliation Annali di Stomatologia 2016;VII (1-2): 4-10
Fracture resistance of endodontically treated teeth restored with a bulkfill flow able material and a resin composite
(e.g., employment, direct payment, stock holdings, retainers, consultant ships, patent licensing arrangements or honoraria), or involvement with any commercial organization with direct financial interest in the subject or materials discussed in this manuscript, nor have any such arrangements existed in the past three years. Any other potential conflict of interest is disclosed.
Meyenberg K. The ideal restoration of endodontically treated teeth - structural and esthetic considerations: a review of the literature and clinical guidelines for the restorative clinician. Eur J Esthet Dent. 2013;8(2):238-268. Steele A, Johnson BR. In vitro fracture strength of endodontically treated premolars. J Endod. 1999;25:6-8. Krejci I, Duc O, Dietschi D, de Campos E. Marginal adaptation, retention and fracture resistance of adhesive composite restorations on devital teeth with and without posts. Oper Dent. 2003;28:127-135. Reeh ES, Messer HH, Douglas WH. Reduction in tooth stiffness as a result of endodontic and restorative procedures. J Endod. 1989;15:512-516. Owen CP. Factors influencing the retention and resistance of preparations for cast intracoronal restorations. J Prosthet Dent. 1986;55(6) 674-677. Fokkinga WA, Kreulen CM, Vallittu PK, Creugers NH. A structured analysis of in vitro failure loads and failure modes of fiber, metal, and ceramic post-and-core systems. Int J Prosthodont. 2004;17:476-482. Panitvisai P, Messer HH. Cuspal deflection in molars in relation to endodontic and restorative procedures. J Endod. 1995;21(2):57-61. Mondelli J, Steagall L, Ishikiriama A, de Lima Navarro MF, Soares FB. Fracture strength of human teeth with cavity preparations. J Prosthet Dent. 1980;43:419-422. Tang W, Wu Y, Smales RJ. Identifying and reducing risks for potential fractures in endodontically treated teeth. J Endod. 2010;36:609-617. Ree M, Schwartz RS. The endo-restorative interface: Current concepts. Dent Clin North Am. 2010;54:345-374. Huang TJ, Shilder H, Nathason D. Effects of moisture content and endodontic treatment on some mechanical properties of human dentin. J Endo. 1992;18:209-215. Tzimpoulas NE, Alisafis MG, Tzanetakis GN, Kontakiotis EG. A prospective study of the extraction and retention incidence of endodontically treated teeth with uncertain prognosis after endodontic referral. J Endod. 2012;38:1326-1329. Ichim I, Kuzmanovic DV, Love RM. A ﬁnite element analysis of ferrule design on restoration resistance and distribution of stress within a root. Int Endod J. 2006;39:443452. Libman WJ, Nicholls JI. Load fatigue of teeth restored with cast posts and cores and complete crowns. Int J Prosthodont. 1995;8:155-161. Akkayan B. An in vitro study evaluating the effect of ferrule length on fracture resistance of endodontically treated teeth restored with ﬁber-reinforced and Zirconia dowel systems. J Prosthet Dent. 2004;92:155-162. Kishen A, Kumar GV, Chen NN. Stress-strain response in human dentine: rethinking fracture predilection in postcore restored teeth. Dent Traumatol. 2004;20:90-100. Da Silva NR, Raposo LH, Versluis A, Fernandes-Neto AJ, Soares CJ. The effect of post, core, crown type, and ferrule presence on the biomechanical behavior of endodontically
Annali di Stomatologia 2016;VII (1-2): 4-10
28. 29. 30. 31. 32.
36. 37. 38.
treated bovine anterior teeth. J Prosthet Dent. 2010;104:306317. Dietschi D, Scampa U, Campanile G, Holz J. Marginal adaptation and seal of direct and indirect Class II composite resin restorations: an in vitro evaluation. Quintessence Int. 1995;26:127-138. Furness A, Tadros MY, Looney SW, Rueggeberg FA. Effect of bulk/incremental fill on internal gap formation of bulk-fill composites. J Dent. 2014;42(4):439-449. Lindberg A, van Dijken JW, Lindberg M. Nine-year evaluation of a polyacid-modified resin composite/resin composite open sandwich technique in Class II cavities. J Dent. 2007;35(2):124-129. Aguiar FH, Ajudarte KF, Lovadino JR. Effect of light curing modes and filling techniques on microleakage of posterior resin composite restorations. Oper Dent. 2002;27(6):557-562. Ruyter IE, Oysaed H. Conversion in different depths of ultraviolet and visible light activated composite materials. Acta Odontol Scand. 1982;40:179-192. Ferracane JL, Mitchem JC, Condon JR, Todd R. Wear and marginal breakdown of composites with various degrees of cure. J Dent Res. 1997;76:1508-1516. Poskus LT, Placido E, Cardoso PE. Inﬂuence of placement techniques on Vickers and Knoop hardness of class II composite resin restorations. Dent Mater. 2004;20:726-732. Sideridou ID, Achilias DS. Elution study of unreacted BisGMA, TEGDMA, UDMA, and Bis-EMA from light-cured dental resins and resin composites using HPLC. J Biomed Mater Res B Appl Biomater. 2005;74:617-626. Musanje L, Darvell BW. Curing-light attenuation in ﬁlled-resin restorative materials. Dental Materials. 2006;22:804-817. Ferracane JL, Greener EH. The effect of resin formulation on the degree of conversion and mechanical properties of dental restorative resin. Journal of Biomedical Materials Research. 1986;20:121-131. Quixﬁl Scientiﬁc Compendium. Dentsply DeTrey; 2003. Sureﬁl SDR ﬂow Directions For Use. Dentsply Caulk; 2009. Venus Bulk Fill Product Proﬁle. Heraeus Kulzer; 2011. Tetric Evo Ceram Bulk Fill Press Release. Ivoclar Vivadent; 2011. Ilie N, Hicke lR. Investigations on a methacrylate-based ﬂowable composite based on the SDR technology. Dental Materials. 2011;27:348-355. Carrilho MR, Tay FR, Pashley DH, Tjäderhane L, Carvalho RM. Mechanical stability of resin-dentin bond components. Dent Mater. 2005;21(3):232-241. Schneider SW. A comparison of canal preparations in straight and curved root canals. Oral Surg Oral Med Oral Pathol. 1971; 32:271-275. Plotino G, Buono L, Grande NM, Lamorgese V, Somma F. Fracture resistance of endodontically treated molars restored with extensive composite resin restorations. J Prosthet Dent. 2008;99(3):225-232. Asundi A, Kishen A. Digital photoelastic investigations on the tooth-bone interface. J Biomed Opt. 2001;6:224-230. Sedgley CM, Messer HH. Are endodontically treated teeth more brittle? J Endod. 1992;18:332-335. Korasli D, Ziraman F, Ozyurt P, Cehreli SB. Microleakage of self-etch primer/adhesives in endodontically treated teeth. J Am Dent Assoc. 2007;138(5):634-640. Galvan RR Jr, West LA, Liewehr FR, Pashley DH. Coronal microleakage of five materials used to create an intracoronal seal in endodontically treated teeth. J Endod. 2002; 28(2):59- 61. Gencoglu N, Pekiner FN, Gumru B, Helvacioglu D. Periapical status and quality of root fillings and coronal restorations in an adult Turkish subpopulation. Eur J Dent. 2010;4(1):1722.
A. Isufi et al.
42. Fathi B, Bahcall J, Maki JS. An in vitro comparison of bacterial leakage of three common restorative materials used as an intracoronal barrier. J Endod. 2007;33(7):872-874. 43. Carvalho RM, Pereira JC, Yoshiyama M, Pashley DH. A review of polymerization contraction: the influence of stress development versus stress relief. Oper Dent. 1996;21(1):1724. 44. Braga RR, Ballester RY, Ferracane JL. Factors involved in the development of polymerization shrinkage stress in resincomposites: a systematic review. Dent Mater. 2005;21: 962-970. 45. Leprince JG, Palin WM, Vanacker J, Sabbagh J, Devaux J, Leloup G. Physico-mechanical characteristics of commercially available bulk-fill composites. J Dent. 2014;42(8):9931000.
46. Lohbauer U, Horst T, Frankenberger R, Kramer N, Petschelt A. Flexural fatigue behaviour of resin composite dental restoratives. Dent Mater. 2003;19:435-440. 47. Lohbauer U, Frankenberger R, Kramer N, Petschelt A. Strength and fatigue performance versus filler fraction of different type of direct dental restoratives. J Biomed Mater Res Part B: Appl Biomater. 2006;76:114-120. 48. Atiyah AH, Baban LM. Fracture resistance of endodontically treated premolars with extensive MOD cavities restored with different composite restorations (An In vitro study). J Bagh Coll Dentistry. 2014;26(1):7-15. 49. Hansen EK, Asmussen E. Cusp fracture of endodontically treated posterior teeth restored with amalgam: teeth restored in Denmark before 1975 versus after 1979. Acta Odontol Scand. 1993;51:73-77.
Annali di Stomatologia 2016;VII (1-2): 4-10